PHYSICAL REVIEW B 78, 153201 共2008兲

Nuclear magnetic resonance linewidth and spin diffusion in

29

Si isotopically controlled silicon

Hiroshi Hayashi and Kohei M. Itoh* Department of Applied Physics and Physico-Informatics, Keio University, 3-14-1 Hiyoshi, Kohoku-ku, Yokohama 223-8522, Japan

Leonid S. Vlasenko A. F. Ioffe Physico–Technical Institute, 194021 Saint Petersburg, Russia 共Received 21 February 2008; revised manuscript received 3 September 2008; published 6 October 2008兲 A nuclear magnetic resonance 共NMR兲 study was performed with n-type silicon single crystals containing Si isotope abundance f ranges from 1.2% to 99.2%. The nuclear spin diffusion coefficient D has been determined from the linewidth of significantly enhanced 29Si NMR signals utilizing a developed dynamic nuclear polarization 共DNP兲 method. The 29Si NMR linewidth depends linearly on f, at least when f ⬍ 10%, and approaches ⬀f 1/2 dependence when f ⬎ 50%. The estimated 29Si nuclear spin diffusion time Tsd between phosphorus atoms used for DNP is more than ten times shorter than the nuclear polarization time T1p of 29Si nuclei around phosphorus. Therefore, the regime of “rapid spin diffusion” is realized in the DNP experiments. 29

DOI: 10.1103/PhysRevB.78.153201

PACS number共s兲: 75.40.Gb, 28.60.⫹s, 76.60.⫺k, 76.70.Fz

The advantages in the availability of silicon based structures with controlled isotope positioning1–4 provide an opportunity for future applications of these semiconductor materials for spin electronics and quantum computing.5,6 This stimulated magnetic resonance investigations including nuclear magnetic resonance 共NMR兲,7 optical nuclear polarization,8 and dynamic nuclear polarization 共DNP兲9,10 in isotopically controlled silicon crystals. Nuclear spin diffusion plays an important role in all these phenomena to transfer the nuclear spin polarization from the local paramagnetic centers to the whole crystal volume. The concept of nuclear spin diffusion was introduced by Bloembergen11 to explain several orders of disagreement between theoretical and experimental values of the nuclear spin-lattice relaxation time T1 in crystals containing paramagnetic centers. The origin of spin diffusion is a dipolar coupling between nuclear magnetic moments. For two nuclear spins, Ii and I j, separated by distance rij, the Hamiltonian Hdd is given by Hdd = dij关4IizI jz − 共Ii+I j− + Ii−I j+兲兴,

共1兲

where Iz is the z component of the angular momentum operator, and I+ and I− are the raising and lowering operators, respectively. The coefficient dij is given by dij =

␥ 2ប 2 共1 – 3 cos3 ij兲, 4兩rij兩3

共2兲

where ␥ is the nuclear gyromagnetic ratio, ប = h / 2 is Planck’s constant, and ij is the angle between the vector rij and the direction of the magnetic field. The energy conserving mutual flip-flop transitions between antiparallel nuclear spins caused by terms Ii+I j− and Ii−I j+ in Eq. 共1兲 are responsible for nuclear spin diffusion. The same interactions described by Hamiltonian 共1兲 provide the contribution to the NMR linewidth ⌬dd and determine the nuclear spin-spin relaxation time T2 ⬇ 1 / ⌬dd. The spin diffusion coefficient is given as11 1098-0121/2008/78共15兲/153201共4兲

D = a2W12 ,

共3兲

where a is the average distance between two neighboring nuclei and W12 is the probability of the flip-flop transition, which can be relatively large for the neighboring nuclei. W12 is of the order of 1 / T2. Because the time T2 is determined by interactions not only between neighboring nuclei but also with the distant nuclei, D is often described by the following approximate relation:12 D⬇

1 2 ⌬dd 2 a ⬇ a . 30 30T2

共4兲

Various theoretical calculations of nuclear spin diffusion based on density-matrix technique,13 on the calculation of higher moments of a resonance line,14 on the statistical mechanics of irreversible processes,15 and on classical spin dynamics16 have been performed. Direct experimental determination of D is limited by the difficulty to create the spatial gradient of the magnetization on the diffusion length L ⬇ 冑DT1. Zhang and Cory17 successfully made a direct measurement of the spin diffusion rate in CaF2 single crystal using incoherent NMR scattering measurements, showing good agreement with theoretical predictions. However, indirect determination of D from time T2 is reliable when dipolar interactions dominate. DNP is a useful tool for the investigation of nuclear spin properties through NMR. DNP in silicon has been carried out recently in lower-temperature and higher-magnetic-field regions to achieve high nuclear polarization.8,18 This Brief Report describes experiments on detecting NMR signals enhanced strongly by a developed DNP technique in silicon single crystals containing different percentages of 29Si isotope f. The analysis of the NMR linewidth with respect to estimation of the diffusion coefficient according to Eq. 共4兲 will be given. Experimental results will be discussed with theoretical calculations of the resonance line shape,19,20 linewidth,20 and diffusion coefficient21 as functions of f using statistical methods for disordered or randomly distributed magnetic moments. The experiments were performed with n-type silicon

153201-1

©2008 The American Physical Society

PHYSICAL REVIEW B 78, 153201 共2008兲

BRIEF REPORTS

TABLE I. Experimentally determined square root of the second moment 共in hertz兲 and the ratio of the higher-order moment to the second moment of the NMR absorption line. Ratios expected for different line shapes are shown for comparison.

NMR Intensity (a.u.)

1%

Sample

M 1/2 2

M 4 / M 22

M 6 / M 32

M 8 / M 42

29

61.1 127 204 436 552

11.1 7.28 4.67 2.66 2.52 ⬁ 3 1.8 1

259 79.9 31.6 12.8 11.2 ⬁ 15 3.9 1

7640 1010 258 99.3 74.2 ⬁ 105 9.0 1

Si-1% Si-5% 29 Si-10% 29 Si-50% 29 Si-100% Lorentzian limit Gaussian Rectangular Pair limit 29

x30

5% 10% 50%

x3

100%

x3

-1500 -1000 -500

0

500 1000 1500

Frequency ν (Hz) FIG. 1. The DNP enhanced 29Si NMR spectra detected in isotopically controlled silicon single crystals for orientation of the magnetic field approximately along 关111兴 crystal axis. The horizontal axis is offset by 29Si nuclear Larmor frequency of 60 MHz; the vertical axis is arbitrary. The thermal equilibrium signal in a 29 Si-5% sample is also shown 共horizontal axis is arbitrarily shifted兲. The dotted curves in the 29Si-50% and 100% samples indicate the components of absorption curve obtained by fitting it with multiple Gaussian curves. The total area under the NMR spectra is normalized to be unity 共but multiplied to present their shapes clearly兲.

single crystals containing 29Si isotopic abundance f of 1.2%, 4.7%, 10.3%, 47.9%, and 99.2% with the phosphorus concentrations Nd = 共0.6– 1.6兲 ⫻ 1015 cm−3 共referred in this text as 29Si-1%, 5%, 10%, 50%, and 100% samples, respectively兲. The weak 29Si NMR signals were enhanced by DNP performed in an EPR JEOL JES-RE3X X-band continuouswave spectrometer. One of the two phosphorus EPR lines was saturated by a 200-mW microwave field at 12 K.9 After 20 h of saturation, the sample was transferred to a Chemagnetics CMX300 CP/MAS-NMR spectrometer where the 29Si NMR signal was detected at room temperature and a magnetic field of 7 T. The absorption spectrum was acquired after Fourier transformation of the free-induction decay signal following a / 2 pulse. The pulse length and acquisition delay time were 9 and 35 s, respectively. The extremely long T1 for all investigated samples 共T1 ⬇ 3 h at room temperature22兲 allowed us to transfer the samples without losing nuclear magnetization. Typical DNP enhanced 29Si NMR spectra are shown in Fig. 1. The thermal equilibrium signal for the 29Si-5% sample detected after 66 h relaxation at room temperature and 7 T is also shown to illustrate the efficiency of DNP. As shown in the theoretical calculations of the resonance line,20

line shape, and width of the DNP enhanced NMR spectra show a strong dependence on the amount of 29Si isotope f and provide a clear observation of the satellite peaks, socalled Pake’s doublet, arising from the nearest-neighbor 29Si nuclei even in a naturally abundant 29Si-5% sample which contains only f 2 = 0.22% of the 29Si pairs in the silicon matrix. In addition, the positions of the satellite peaks depend on the crystal orientation in the external magnetic field described by Eq. 共2兲.7,23 Although the lines have a partially overlapped structure, the components of the absorption curve in 29Si-50% and 100% samples are Gaussian and well fitted with multiple Gaussian curves. The method of moments developed by Van Vleck24 is often used for the analysis of the resonance line shape. The 2nth moment M 2n and the ratio of the higher-order moment to the second moment M 2n / M n2 are commonly used as standard parameters for the characterization.19 A sharp doublet peak 共two ␦ functions at = ⫾ M 1/2 2 兲 corresponds to M 2n / M n2 = 1 共pair limit兲, while the double peak merges into a single peak when M 4 / M 22 ⱖ 2.85. Gaussian line shape has M 4 / M 22 = 3. For a narrow line shape with longer wings, such as a Lorentzian, M 2n / M n2 → ⬁ 共Lorentzian limit兲. The spectral moments were numerically calculated from the experimental NMR lines 共Table I兲. We can quantitatively see how the NMR line shape varies from a single Lorentzian in a 29 Si-1% sample to a double peak in a 29Si-100% sample with an increase in 29Si abundance. It should be noted that the analysis of the linewidth using the second and fourth moments of the Gaussian and Lorentzian line shapes shows the linear dependence of linewidth on f when f ⬍ 1% and square-root dependence when f ⬎ 10%.25 To estimate the linewidths ⌬ of the detected NMR signals of the complex line shapes, we used the values of ⌬ determined in Ref. 20 as ⌬ = 1/F共0兲,

共5兲

where F共0兲 is the value of the normalized line-shape function F共兲 taken at the center of the NMR line 共 = 0 Hz兲. The NMR linewidths ⌬ obtained by this method from the experimentally observed signals at the orientation of the mag-

153201-2

PHYSICAL REVIEW B 78, 153201 共2008兲

1000 500 0

0

20

40 29

60

80

100

Si Abundance f (%)

FIG. 2. Dependence of the NMR linewidth ⌬ determined by Eq. 共5兲 共squares兲 and FWHM 共circles兲 on the 29Si isotope abundance f.

NMR Linewidth ∆νdd (Hz)

netic field approximately along 关111兴 crystal axis are plotted in Fig. 2 as a function of f 共squares兲. The full widths at half maximum 共FWHM兲 measured directly from the NMR lines are also plotted in Fig. 2 共circles兲. The NMR linewidth due to the dipole-dipole interaction between nuclear magnetic moments should vanish at infinite nuclear spin spacing rij. However, ⌬ goes to a nonzero value of ⬃70 Hz at f = 0% 共see Fig. 2兲. The remaining linewidth of 70 Hz shows some additional contribution to FWHM, such as inhomogeneity of the external magnetic field over the sample and a nonzero delay time of the NMR spectrometer when the strongest part of the free-induction decay signal is lost. To obtain the contribution to linewidth purely due to the dipole-dipole interaction, ⌬dd, the value of 70 Hz was subtracted from ⌬. The dependence of the ⌬dd = ⌬ − 70 Hz on f is shown in Fig. 3. These results show that ⌬dd determined by different methods linearly depends on f when f ⬍ 10% and changes to square-root dependence when f ⬎ 50%, which is in good agreement with the theoretical calculations of the linewidth in the system of randomly distributed spins.20 In addition, we estimated the nuclear diffusion coefficient D using Eq. 共4兲 and values of ⌬dd. The average distance between 29Si nuclei a can be found from the relation, 3000 1000

f 100

10

f

2

1500

5

-14

cm /s)

2000

4

Diffusion Coefficient D (10

NMR Linewidth ∆ν (Hz)

BRIEF REPORTS

3 2 1 0

0

29

60

80

100

Si Abundance f (%)

FIG. 4. Dependence of the 29Si nuclear-spin-diffusion coefficient D on the 29Si isotope abundance f.

冉 冊

−1/3 a ⬇ NN = f

8 d3

−1/3

共6兲

,

where NN is the 29Si concentration, 8 is the number of atoms in a unit cell of diamond structure, and d = 0.543 nm is the lattice constant of silicon. The dependence of D on f is shown in Fig. 4. The ⌬dd values were taken using Eq. 共5兲. A monotonous increase in D with an increase in f and a slow increase at higher abundance is in qualitative agreement with the theoretical simulation of spin diffusion in a disordered spin system.21 Similar dependence of D on f was found for the FWHM estimations. Using the values of D, the diffusion time Tsd of the nuclear polarization transfer on the distance of L = R / 2 between paramagnetic centers can be found, Tsd ⬇

L2 R2 = , D 4D

共7兲

where R ⬇ N−1/3 is the average distance between phosphorus d atoms. The distances a and L, and time Tsd for the investigated samples are summarized in Table II. The time Tsd can be compared with the nuclear spin polarization time T1p obtained from the exponential growth of 29 Si NMR signals in the DNP experiments and are also listed in Table II. The time Tsd is much shorter than the nuclear polarization time showing the fast 29Si nuclear spin diffusion between the phosphorus paramagnetic centers. Together with the observed exponential increase in the nuclear polarization with the saturation time, it allows us to conclude that the TABLE II. The average distance between 29Si nuclei a 共Å兲, average half distance between phosphorus donors L 共Å兲, nuclear spin diffusion time Tsd 共hours兲, and nuclear spin polarization time T1p 共hours兲 in the investigated samples. Sample

10

40 29

1/2

1

1

20

a

L

Tsd

T1p

12 7.5 5.8 3.5 2.7

560 540 430 590 540

0.82 0.47 0.25 0.24 0.19

73.5 19.5 4.5 8.8 9.3

100 29

Si Abundance f (%)

Si-1% Si-5% 29 Si-10% 29 Si-50% 29 Si-100% 29

FIG. 3. Dependence of the NMR linewidth due to the dipoledipole interaction, ⌬dd, determined by Eq. 共5兲 共squares兲 and FWHM 共circles兲 on the 29Si isotope abundance f. The dashed lines show the linear and square-root dependences.

153201-3

PHYSICAL REVIEW B 78, 153201 共2008兲

BRIEF REPORTS

case of rapid nuclear spin diffusion regime12,26–28 is realized in all investigated samples. In summary, the analysis of the 29Si NMR linewidth in the silicon crystals containing different amounts of the 29Si isotope showed that the NMR linewidth is proportional to f when f ⬍ 10% and approaches square-root dependence on f when f ⬎ 50%. The nuclear spin diffusion coefficient D increased from 1 ⫻ 10−14 to 4 ⫻ 10−14 cm2 / s. The nuclear-spin diffusion between phosphorus atoms is more than ten times faster than the increase in the 29Si nuclear polarization around phosphorus atoms in the DNP experiments corre-

*[email protected] 1 K.

Takyu, K. M. Itoh, K. Oka, N. Saito, and V. I. Ozhogin, Jpn. J. Appl. Phys., Part 2 38, L1493 共1999兲. 2 T. Kojima, R. Nebashi, K. M. Itoh, and Y. Shiraki, Appl. Phys. Lett. 83, 2318 共2003兲. 3 K. M. Itoh, J. Kato, F. Uemura, A. K. Kaliteyevskii, O. N. Godisov, G. G. Devyatych, A. D. Bulanov, A. V. Gusev, I. D. Kovalev, P. G. Sennikov, H.-J. Pohl, N. V. Abrosimov, and H. Riemann, Jpn. J. Appl. Phys., Part 1 42, 62481 共2003兲. 4 T. Sekiguchi, S. Yoshida, and K. M. Itoh, Phys. Rev. Lett. 95, 106101 共2005兲. 5 T. D. Ladd, J. R. Goldman, F. Yamaguchi, Y. Yamamoto, E. Abe, and K. M. Itoh, Phys. Rev. Lett. 89, 017901 共2002兲. 6 K. M. Itoh, Solid State Commun. 133, 747 共2005兲. 7 A. S. Verhulst, D. Maryenko, Y. Yamamoto, and K. M. Itoh, Phys. Rev. B 68, 054105 共2003兲. 8 A. S. Verhulst, I. G. Rau, Y. Yamamoto, and K. M. Itoh, Phys. Rev. B 71, 235206 共2005兲. 9 H. Hayashi, W. Ko, T. Itahashi, A. Sagara, K. M. Itoh, L. S. Vlasenko, and M. P. Vlasenko, Phys. Status Solidi C 3, 4388 共2006兲. 10 L. S. Vlasenko, M. P. Vlasenko, D. S. Poloskin, R. Laiho, H. Hayashi, T. Itahashi, A. Sagara, and K. M. Itoh, Phys. Status

sponding to the regime of the rapid spin diffusion. We thank T. Itahashi for all the helpful experimental support. We also thank Central Service Facilities for Research at Keio University for the provision of the well-developed experimentation environment. This work was supported in part by Grant-in-Aid for Scientific Research by MEXT Specially Promoted Research No. 18001002, by Special Coordination Funds for Promoting Science and Technology, and by Grantin-Aid for the Global Center of Excellence at Keio University.

Solidi C 3, 4376 共2006兲. Bloembergen, Physica 共Amsterdam兲 15, 386 共1949兲. 12 G. R. Khutsishvili, Sov. Phys. Usp. 8, 743 共1966兲. 13 I. J. Lowe and S. Gade, Phys. Rev. 156, 817 共1967兲. 14 A. G. Redfield and W. N. Yu, Phys. Rev. 169, 443 共1968兲. 15 P. Borckmans and D. Walgraef, Phys. Rev. 167, 282 共1968兲. 16 C. Tang and J. S. Waugh, Phys. Rev. B 45, 748 共1992兲. 17 W. Zhang and D. G. Cory, Phys. Rev. Lett. 80, 1324 共1998兲. 18 A. E. Dementyev, D. G. Cory, and C. R. Ramanathan, Phys. Rev. Lett. 100, 127601 共2008兲. 19 G. W. Parker and F. Lado, Phys. Rev. B 8, 3081 共1973兲. 20 C. W. Myles, C. Ebner, and P. A. Fedders, Phys. Rev. B 14, 1 共1976兲. 21 I. M. Nolden and R. J. Silbey, Phys. Rev. B 54, 381 共1996兲. 22 R. G. Shulman and B. J. Wyluda, Phys. Rev. 103, 1127 共1956兲. 23 L. S. Vlasenko, Sov. Phys. Tech. Phys. 10, 467 共1984兲. 24 J. H. Van Vleck, Phys. Rev. 74, 1168 共1948兲. 25 C. Kittel and E. Abrahams, Phys. Rev. 90, 238 共1953兲. 26 W. E. Blumberg, Phys. Rev. 119, 79 共1960兲. 27 A. Abragam, The Principles of Nuclear Magnetism 共Oxford University Press, New York, 1961兲. 28 C. D. Jeffries, Dynamic Nuclear Orientation 共Wiley, New York, 1963兲. 11 N.

153201-4

Nuclear magnetic resonance linewidth and spin diffusion in

29

Si isotopically controlled silicon

Hiroshi Hayashi and Kohei M. Itoh* Department of Applied Physics and Physico-Informatics, Keio University, 3-14-1 Hiyoshi, Kohoku-ku, Yokohama 223-8522, Japan

Leonid S. Vlasenko A. F. Ioffe Physico–Technical Institute, 194021 Saint Petersburg, Russia 共Received 21 February 2008; revised manuscript received 3 September 2008; published 6 October 2008兲 A nuclear magnetic resonance 共NMR兲 study was performed with n-type silicon single crystals containing Si isotope abundance f ranges from 1.2% to 99.2%. The nuclear spin diffusion coefficient D has been determined from the linewidth of significantly enhanced 29Si NMR signals utilizing a developed dynamic nuclear polarization 共DNP兲 method. The 29Si NMR linewidth depends linearly on f, at least when f ⬍ 10%, and approaches ⬀f 1/2 dependence when f ⬎ 50%. The estimated 29Si nuclear spin diffusion time Tsd between phosphorus atoms used for DNP is more than ten times shorter than the nuclear polarization time T1p of 29Si nuclei around phosphorus. Therefore, the regime of “rapid spin diffusion” is realized in the DNP experiments. 29

DOI: 10.1103/PhysRevB.78.153201

PACS number共s兲: 75.40.Gb, 28.60.⫹s, 76.60.⫺k, 76.70.Fz

The advantages in the availability of silicon based structures with controlled isotope positioning1–4 provide an opportunity for future applications of these semiconductor materials for spin electronics and quantum computing.5,6 This stimulated magnetic resonance investigations including nuclear magnetic resonance 共NMR兲,7 optical nuclear polarization,8 and dynamic nuclear polarization 共DNP兲9,10 in isotopically controlled silicon crystals. Nuclear spin diffusion plays an important role in all these phenomena to transfer the nuclear spin polarization from the local paramagnetic centers to the whole crystal volume. The concept of nuclear spin diffusion was introduced by Bloembergen11 to explain several orders of disagreement between theoretical and experimental values of the nuclear spin-lattice relaxation time T1 in crystals containing paramagnetic centers. The origin of spin diffusion is a dipolar coupling between nuclear magnetic moments. For two nuclear spins, Ii and I j, separated by distance rij, the Hamiltonian Hdd is given by Hdd = dij关4IizI jz − 共Ii+I j− + Ii−I j+兲兴,

共1兲

where Iz is the z component of the angular momentum operator, and I+ and I− are the raising and lowering operators, respectively. The coefficient dij is given by dij =

␥ 2ប 2 共1 – 3 cos3 ij兲, 4兩rij兩3

共2兲

where ␥ is the nuclear gyromagnetic ratio, ប = h / 2 is Planck’s constant, and ij is the angle between the vector rij and the direction of the magnetic field. The energy conserving mutual flip-flop transitions between antiparallel nuclear spins caused by terms Ii+I j− and Ii−I j+ in Eq. 共1兲 are responsible for nuclear spin diffusion. The same interactions described by Hamiltonian 共1兲 provide the contribution to the NMR linewidth ⌬dd and determine the nuclear spin-spin relaxation time T2 ⬇ 1 / ⌬dd. The spin diffusion coefficient is given as11 1098-0121/2008/78共15兲/153201共4兲

D = a2W12 ,

共3兲

where a is the average distance between two neighboring nuclei and W12 is the probability of the flip-flop transition, which can be relatively large for the neighboring nuclei. W12 is of the order of 1 / T2. Because the time T2 is determined by interactions not only between neighboring nuclei but also with the distant nuclei, D is often described by the following approximate relation:12 D⬇

1 2 ⌬dd 2 a ⬇ a . 30 30T2

共4兲

Various theoretical calculations of nuclear spin diffusion based on density-matrix technique,13 on the calculation of higher moments of a resonance line,14 on the statistical mechanics of irreversible processes,15 and on classical spin dynamics16 have been performed. Direct experimental determination of D is limited by the difficulty to create the spatial gradient of the magnetization on the diffusion length L ⬇ 冑DT1. Zhang and Cory17 successfully made a direct measurement of the spin diffusion rate in CaF2 single crystal using incoherent NMR scattering measurements, showing good agreement with theoretical predictions. However, indirect determination of D from time T2 is reliable when dipolar interactions dominate. DNP is a useful tool for the investigation of nuclear spin properties through NMR. DNP in silicon has been carried out recently in lower-temperature and higher-magnetic-field regions to achieve high nuclear polarization.8,18 This Brief Report describes experiments on detecting NMR signals enhanced strongly by a developed DNP technique in silicon single crystals containing different percentages of 29Si isotope f. The analysis of the NMR linewidth with respect to estimation of the diffusion coefficient according to Eq. 共4兲 will be given. Experimental results will be discussed with theoretical calculations of the resonance line shape,19,20 linewidth,20 and diffusion coefficient21 as functions of f using statistical methods for disordered or randomly distributed magnetic moments. The experiments were performed with n-type silicon

153201-1

©2008 The American Physical Society

PHYSICAL REVIEW B 78, 153201 共2008兲

BRIEF REPORTS

TABLE I. Experimentally determined square root of the second moment 共in hertz兲 and the ratio of the higher-order moment to the second moment of the NMR absorption line. Ratios expected for different line shapes are shown for comparison.

NMR Intensity (a.u.)

1%

Sample

M 1/2 2

M 4 / M 22

M 6 / M 32

M 8 / M 42

29

61.1 127 204 436 552

11.1 7.28 4.67 2.66 2.52 ⬁ 3 1.8 1

259 79.9 31.6 12.8 11.2 ⬁ 15 3.9 1

7640 1010 258 99.3 74.2 ⬁ 105 9.0 1

Si-1% Si-5% 29 Si-10% 29 Si-50% 29 Si-100% Lorentzian limit Gaussian Rectangular Pair limit 29

x30

5% 10% 50%

x3

100%

x3

-1500 -1000 -500

0

500 1000 1500

Frequency ν (Hz) FIG. 1. The DNP enhanced 29Si NMR spectra detected in isotopically controlled silicon single crystals for orientation of the magnetic field approximately along 关111兴 crystal axis. The horizontal axis is offset by 29Si nuclear Larmor frequency of 60 MHz; the vertical axis is arbitrary. The thermal equilibrium signal in a 29 Si-5% sample is also shown 共horizontal axis is arbitrarily shifted兲. The dotted curves in the 29Si-50% and 100% samples indicate the components of absorption curve obtained by fitting it with multiple Gaussian curves. The total area under the NMR spectra is normalized to be unity 共but multiplied to present their shapes clearly兲.

single crystals containing 29Si isotopic abundance f of 1.2%, 4.7%, 10.3%, 47.9%, and 99.2% with the phosphorus concentrations Nd = 共0.6– 1.6兲 ⫻ 1015 cm−3 共referred in this text as 29Si-1%, 5%, 10%, 50%, and 100% samples, respectively兲. The weak 29Si NMR signals were enhanced by DNP performed in an EPR JEOL JES-RE3X X-band continuouswave spectrometer. One of the two phosphorus EPR lines was saturated by a 200-mW microwave field at 12 K.9 After 20 h of saturation, the sample was transferred to a Chemagnetics CMX300 CP/MAS-NMR spectrometer where the 29Si NMR signal was detected at room temperature and a magnetic field of 7 T. The absorption spectrum was acquired after Fourier transformation of the free-induction decay signal following a / 2 pulse. The pulse length and acquisition delay time were 9 and 35 s, respectively. The extremely long T1 for all investigated samples 共T1 ⬇ 3 h at room temperature22兲 allowed us to transfer the samples without losing nuclear magnetization. Typical DNP enhanced 29Si NMR spectra are shown in Fig. 1. The thermal equilibrium signal for the 29Si-5% sample detected after 66 h relaxation at room temperature and 7 T is also shown to illustrate the efficiency of DNP. As shown in the theoretical calculations of the resonance line,20

line shape, and width of the DNP enhanced NMR spectra show a strong dependence on the amount of 29Si isotope f and provide a clear observation of the satellite peaks, socalled Pake’s doublet, arising from the nearest-neighbor 29Si nuclei even in a naturally abundant 29Si-5% sample which contains only f 2 = 0.22% of the 29Si pairs in the silicon matrix. In addition, the positions of the satellite peaks depend on the crystal orientation in the external magnetic field described by Eq. 共2兲.7,23 Although the lines have a partially overlapped structure, the components of the absorption curve in 29Si-50% and 100% samples are Gaussian and well fitted with multiple Gaussian curves. The method of moments developed by Van Vleck24 is often used for the analysis of the resonance line shape. The 2nth moment M 2n and the ratio of the higher-order moment to the second moment M 2n / M n2 are commonly used as standard parameters for the characterization.19 A sharp doublet peak 共two ␦ functions at = ⫾ M 1/2 2 兲 corresponds to M 2n / M n2 = 1 共pair limit兲, while the double peak merges into a single peak when M 4 / M 22 ⱖ 2.85. Gaussian line shape has M 4 / M 22 = 3. For a narrow line shape with longer wings, such as a Lorentzian, M 2n / M n2 → ⬁ 共Lorentzian limit兲. The spectral moments were numerically calculated from the experimental NMR lines 共Table I兲. We can quantitatively see how the NMR line shape varies from a single Lorentzian in a 29 Si-1% sample to a double peak in a 29Si-100% sample with an increase in 29Si abundance. It should be noted that the analysis of the linewidth using the second and fourth moments of the Gaussian and Lorentzian line shapes shows the linear dependence of linewidth on f when f ⬍ 1% and square-root dependence when f ⬎ 10%.25 To estimate the linewidths ⌬ of the detected NMR signals of the complex line shapes, we used the values of ⌬ determined in Ref. 20 as ⌬ = 1/F共0兲,

共5兲

where F共0兲 is the value of the normalized line-shape function F共兲 taken at the center of the NMR line 共 = 0 Hz兲. The NMR linewidths ⌬ obtained by this method from the experimentally observed signals at the orientation of the mag-

153201-2

PHYSICAL REVIEW B 78, 153201 共2008兲

1000 500 0

0

20

40 29

60

80

100

Si Abundance f (%)

FIG. 2. Dependence of the NMR linewidth ⌬ determined by Eq. 共5兲 共squares兲 and FWHM 共circles兲 on the 29Si isotope abundance f.

NMR Linewidth ∆νdd (Hz)

netic field approximately along 关111兴 crystal axis are plotted in Fig. 2 as a function of f 共squares兲. The full widths at half maximum 共FWHM兲 measured directly from the NMR lines are also plotted in Fig. 2 共circles兲. The NMR linewidth due to the dipole-dipole interaction between nuclear magnetic moments should vanish at infinite nuclear spin spacing rij. However, ⌬ goes to a nonzero value of ⬃70 Hz at f = 0% 共see Fig. 2兲. The remaining linewidth of 70 Hz shows some additional contribution to FWHM, such as inhomogeneity of the external magnetic field over the sample and a nonzero delay time of the NMR spectrometer when the strongest part of the free-induction decay signal is lost. To obtain the contribution to linewidth purely due to the dipole-dipole interaction, ⌬dd, the value of 70 Hz was subtracted from ⌬. The dependence of the ⌬dd = ⌬ − 70 Hz on f is shown in Fig. 3. These results show that ⌬dd determined by different methods linearly depends on f when f ⬍ 10% and changes to square-root dependence when f ⬎ 50%, which is in good agreement with the theoretical calculations of the linewidth in the system of randomly distributed spins.20 In addition, we estimated the nuclear diffusion coefficient D using Eq. 共4兲 and values of ⌬dd. The average distance between 29Si nuclei a can be found from the relation, 3000 1000

f 100

10

f

2

1500

5

-14

cm /s)

2000

4

Diffusion Coefficient D (10

NMR Linewidth ∆ν (Hz)

BRIEF REPORTS

3 2 1 0

0

29

60

80

100

Si Abundance f (%)

FIG. 4. Dependence of the 29Si nuclear-spin-diffusion coefficient D on the 29Si isotope abundance f.

冉 冊

−1/3 a ⬇ NN = f

8 d3

−1/3

共6兲

,

where NN is the 29Si concentration, 8 is the number of atoms in a unit cell of diamond structure, and d = 0.543 nm is the lattice constant of silicon. The dependence of D on f is shown in Fig. 4. The ⌬dd values were taken using Eq. 共5兲. A monotonous increase in D with an increase in f and a slow increase at higher abundance is in qualitative agreement with the theoretical simulation of spin diffusion in a disordered spin system.21 Similar dependence of D on f was found for the FWHM estimations. Using the values of D, the diffusion time Tsd of the nuclear polarization transfer on the distance of L = R / 2 between paramagnetic centers can be found, Tsd ⬇

L2 R2 = , D 4D

共7兲

where R ⬇ N−1/3 is the average distance between phosphorus d atoms. The distances a and L, and time Tsd for the investigated samples are summarized in Table II. The time Tsd can be compared with the nuclear spin polarization time T1p obtained from the exponential growth of 29 Si NMR signals in the DNP experiments and are also listed in Table II. The time Tsd is much shorter than the nuclear polarization time showing the fast 29Si nuclear spin diffusion between the phosphorus paramagnetic centers. Together with the observed exponential increase in the nuclear polarization with the saturation time, it allows us to conclude that the TABLE II. The average distance between 29Si nuclei a 共Å兲, average half distance between phosphorus donors L 共Å兲, nuclear spin diffusion time Tsd 共hours兲, and nuclear spin polarization time T1p 共hours兲 in the investigated samples. Sample

10

40 29

1/2

1

1

20

a

L

Tsd

T1p

12 7.5 5.8 3.5 2.7

560 540 430 590 540

0.82 0.47 0.25 0.24 0.19

73.5 19.5 4.5 8.8 9.3

100 29

Si Abundance f (%)

Si-1% Si-5% 29 Si-10% 29 Si-50% 29 Si-100% 29

FIG. 3. Dependence of the NMR linewidth due to the dipoledipole interaction, ⌬dd, determined by Eq. 共5兲 共squares兲 and FWHM 共circles兲 on the 29Si isotope abundance f. The dashed lines show the linear and square-root dependences.

153201-3

PHYSICAL REVIEW B 78, 153201 共2008兲

BRIEF REPORTS

case of rapid nuclear spin diffusion regime12,26–28 is realized in all investigated samples. In summary, the analysis of the 29Si NMR linewidth in the silicon crystals containing different amounts of the 29Si isotope showed that the NMR linewidth is proportional to f when f ⬍ 10% and approaches square-root dependence on f when f ⬎ 50%. The nuclear spin diffusion coefficient D increased from 1 ⫻ 10−14 to 4 ⫻ 10−14 cm2 / s. The nuclear-spin diffusion between phosphorus atoms is more than ten times faster than the increase in the 29Si nuclear polarization around phosphorus atoms in the DNP experiments corre-

*[email protected] 1 K.

Takyu, K. M. Itoh, K. Oka, N. Saito, and V. I. Ozhogin, Jpn. J. Appl. Phys., Part 2 38, L1493 共1999兲. 2 T. Kojima, R. Nebashi, K. M. Itoh, and Y. Shiraki, Appl. Phys. Lett. 83, 2318 共2003兲. 3 K. M. Itoh, J. Kato, F. Uemura, A. K. Kaliteyevskii, O. N. Godisov, G. G. Devyatych, A. D. Bulanov, A. V. Gusev, I. D. Kovalev, P. G. Sennikov, H.-J. Pohl, N. V. Abrosimov, and H. Riemann, Jpn. J. Appl. Phys., Part 1 42, 62481 共2003兲. 4 T. Sekiguchi, S. Yoshida, and K. M. Itoh, Phys. Rev. Lett. 95, 106101 共2005兲. 5 T. D. Ladd, J. R. Goldman, F. Yamaguchi, Y. Yamamoto, E. Abe, and K. M. Itoh, Phys. Rev. Lett. 89, 017901 共2002兲. 6 K. M. Itoh, Solid State Commun. 133, 747 共2005兲. 7 A. S. Verhulst, D. Maryenko, Y. Yamamoto, and K. M. Itoh, Phys. Rev. B 68, 054105 共2003兲. 8 A. S. Verhulst, I. G. Rau, Y. Yamamoto, and K. M. Itoh, Phys. Rev. B 71, 235206 共2005兲. 9 H. Hayashi, W. Ko, T. Itahashi, A. Sagara, K. M. Itoh, L. S. Vlasenko, and M. P. Vlasenko, Phys. Status Solidi C 3, 4388 共2006兲. 10 L. S. Vlasenko, M. P. Vlasenko, D. S. Poloskin, R. Laiho, H. Hayashi, T. Itahashi, A. Sagara, and K. M. Itoh, Phys. Status

sponding to the regime of the rapid spin diffusion. We thank T. Itahashi for all the helpful experimental support. We also thank Central Service Facilities for Research at Keio University for the provision of the well-developed experimentation environment. This work was supported in part by Grant-in-Aid for Scientific Research by MEXT Specially Promoted Research No. 18001002, by Special Coordination Funds for Promoting Science and Technology, and by Grantin-Aid for the Global Center of Excellence at Keio University.

Solidi C 3, 4376 共2006兲. Bloembergen, Physica 共Amsterdam兲 15, 386 共1949兲. 12 G. R. Khutsishvili, Sov. Phys. Usp. 8, 743 共1966兲. 13 I. J. Lowe and S. Gade, Phys. Rev. 156, 817 共1967兲. 14 A. G. Redfield and W. N. Yu, Phys. Rev. 169, 443 共1968兲. 15 P. Borckmans and D. Walgraef, Phys. Rev. 167, 282 共1968兲. 16 C. Tang and J. S. Waugh, Phys. Rev. B 45, 748 共1992兲. 17 W. Zhang and D. G. Cory, Phys. Rev. Lett. 80, 1324 共1998兲. 18 A. E. Dementyev, D. G. Cory, and C. R. Ramanathan, Phys. Rev. Lett. 100, 127601 共2008兲. 19 G. W. Parker and F. Lado, Phys. Rev. B 8, 3081 共1973兲. 20 C. W. Myles, C. Ebner, and P. A. Fedders, Phys. Rev. B 14, 1 共1976兲. 21 I. M. Nolden and R. J. Silbey, Phys. Rev. B 54, 381 共1996兲. 22 R. G. Shulman and B. J. Wyluda, Phys. Rev. 103, 1127 共1956兲. 23 L. S. Vlasenko, Sov. Phys. Tech. Phys. 10, 467 共1984兲. 24 J. H. Van Vleck, Phys. Rev. 74, 1168 共1948兲. 25 C. Kittel and E. Abrahams, Phys. Rev. 90, 238 共1953兲. 26 W. E. Blumberg, Phys. Rev. 119, 79 共1960兲. 27 A. Abragam, The Principles of Nuclear Magnetism 共Oxford University Press, New York, 1961兲. 28 C. D. Jeffries, Dynamic Nuclear Orientation 共Wiley, New York, 1963兲. 11 N.

153201-4